# Ultrasmall Quantum Dots: A Tool for in Vitro and in Vivo Fluorescence Imaging

Pavel Linkov, Kirill V Vokhmintcev, Pavel S Samokhvalov, Igor Nabiev

► To cite this version:

Pavel Linkov, Kirill V Vokhmintcev, Pavel S Samokhvalov, Igor Nabiev. Ultrasmall Quantum Dots: A Tool for in Vitro and in Vivo Fluorescence Imaging. Journal of Physics: Conference Series, 2017, International Symposium Physics, Engineering and Technologies for Bio-Medicine, 784, pp.012033. 10.1088/1742-6596/784/1/012033. [hal-03036150](https://hal.science/hal-03036150)

HAL Id: hal-03036150

https://hal.science/hal-03036150

Submitted on 2 Dec 2020

HAL is a multi-disciplinary open access
archive for the deposit and dissemination of sci-
entific research documents, whether they are pub-
lished or not. The documents may come from
teaching and research institutions in France or
abroad, or from public or private research centers.

L'archive ouverte pluridisciplinaire HAL, est
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d'enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.

<figure><img src="image_1.png" /></figure>

Distributed under a Creative Commons Attribution 4.0 International License
PAPER • OPEN ACCESS

# Ultrasmall Quantum Dots: A Tool for in Vitro and in Vivo Fluorescence Imaging

To cite this article: Pavel Linkov et al 2017 *J. Phys.: Conf. Ser.* **784** 012033

View the [article online](#) for updates and enhancements.

## Related content

- Perturbation theory of interacting electrons in a quantum dot with hard-wall confinement potential
J O Fjærestad, A Matulis and K A Chao

- Electron-electron interaction in quantum dots
A Matulis, John Ove Fjærestad and K A Chao

<figure><img src="image_2.png" /></figure>

IOP ebooks™

Bringing together innovative digital publishing with leading authors from the global scientific community.

Start exploring the collection-download the first chapter of every title for free.
# Ultrasmall Quantum Dots: A Tool for in Vitro and in Vivo Fluorescence Imaging

Pavel Linkov¹,²,³, Kirill V Vokhmintcev¹, Pavel S Samokhvalov¹, Igor Nabiev¹,³

¹National Research Nuclear University MEPhI (Moscow Engineering Physics Institute), 115409 Moscow, Russian Federation

²Department of Chemistry, Moscow State University, 1 Leninskie gory, 119991 Moscow, Russia

³University of Reims Champagne-Ardenne, 51100 Reims, France

E-mail: valinkov@gmail.com

**Abstract.** Fluorescence bioimaging is an increasingly popular approach in biomedical research and diagnosis, where semiconductor nanocrystals or quantum dots (QDs) have proved to be excellent fluorescent labels. The use of ultrasmall QDs in nanoprobes extends the possibilities of bioimaging owing to an enhanced capacity for penetrating through cell membranes. However, the QDs synthesis is accompanied by the rapid growth of nanocrystals in colloidal medium what prevents obtaining sufficiently small QDs prepared by conventional approaches. Here, a one-pot injection technique of QD synthesis in an organic medium, with the reaction terminated at an early crystal growth stage and excess precursors eliminated by gel permeation chromatography, is proposed. This technique yields defect-free cadmium selenide QD cores about 1.5 nm in size emitting at the wavelengths less than 500 nm. Coating of these QDs with epitaxial shells of different compositions ensures a photoluminescence quantum yield approaching 100%. The resultant ultrasmall QDs are promising components of nanoprobes to be used for imaging intracellular and intranuclear events down to the molecular level.

## 1. Introduction

Quantum dots (QDs) are semiconductor nanocrystals (NCs) several nanometers in size capable of photoluminescence (PL) in a wide spectral range. Their energy structure and characteristics of light absorption and fluorescence strongly depend on the QD size because of the quantum confinement effect [1,2]. Advanced methods of one-pot injection synthesis with one component injected into a hot solution of the other component [3] allow obtaining QDs with controllable sizes and, hence, PL parameters by varying the reaction time, temperature, and/or types of precursors. Core/shell QDs consisting of a fluorescing core (usually, CdSe) and a thin epitaxial inorganic shell of a semiconductor with a higher band gap (usually, CdS or ZnS) emitting in the range from 500 to 650 nm, depending on the core size, are currently the most common type of QDs. The shell enhances charge carrier localization in the core, protects the core from the environment, and suppresses blinking [4,5].

QDs are increasingly widely used in various fields [6,7], including biomedical research and medicine [8,9]. A typical biomedical application of QDs is their use as fluorescent labels, which are advantageous over the routinely used organic dyes due to the unique optical properties and high stability. In this field, the QD shell provides and additional advantage in that it facilitates the

<figure><img src="image_3.png" /></figure>
attachment of hydrophilic ligands to the QD surface to make the QDs water-soluble. These QDs can serve as components of complex suspension microarrays or nanoprobes, whose PL may be excited in either the one-photon [10] or the two-photon [11,12] modes.

In recent years, the possibility of imaging intracellular events down to the molecular level by means of QDs has raised special interest [13]. In this case, of particular importance are small sizes of QDs and the absence of PL blinking [14]. In addition, ultrasmall CdSe cores fluorescing in the blue spectral region are promising components of next-generation light-emitting diodes. Therefore, the development of ultrasmall QDs with a shell effectively enhancing fluorescence is an urgent task.

The main difficulty with obtaining QD cores smaller than 2 nm [15] is that the NC growth at early stages is so rapid that larger crystals are formed almost instantaneously. To date, methods for obtaining the so-called magic-size clusters with a high thermodynamic stability and very narrow optical transitions [16] in the UV and blue spectral regions have been developed. However, this type of NCs is unsuitable for biomedical applications because attempts at coating them with inorganic shells effectively enhancing the PL quantum yield (QY) and protecting the core have thus far failed. Apparently, the reason is that these clusters are structurally different from common QDs [16], which makes the standard coating techniques ineffective.

In this study, we suggest a new procedures for synthesizing CdSe cores with diameters as small as 1.5 nm and coating them with one or several layers of an inorganic shell to obtain CdSe/ZnS and CdSe/ZnS/CdS/ZnS core/shell QDs with highly uniform sizes and a PL QY as high as 90% fluorescing in the region between 480 and 540 nm.

## 2. Results

Our procedure, described in detail elsewhere [17], is based on the high-temperature injection synthesis method. In this study, the growth of QD cores was monitored by recording their absorption and emission spectra. The PL QY was measured relative to Coumarin 102 and fluorescein dyes.

Our first objective was to obtain CdSe NCs of strictly controllable size, which was fulfilled by precise control of the reaction time and removal of all unreacted precursors.

First, we measured the kinetics of NC growth by monitoring the position of the first excitonic transition in the light absorption spectrum, and, by using the relationship between the latter and the NC diameter [18] we plotted an approximated calibration curve. The measurement showed that the reaction had to be terminated within about 45 s to obtain QD cores smaller than 1.5 nm in diameter. However, the commonly used method of terminating the synthesis by cooling the reaction flask with an air flow takes more than 1 min to cool the mixture to a temperature below 100°C, during which time the crystal growth gradually slows down. This leads to size heterogeneity of the resultant NCs.

Therefore, we put the reaction mixture into liquid nitrogen after 45 s of synthesis to stop the reaction instantaneously. The frozen mixture was collected into excess isopropyl alcohol, and when it warmed to room temperature, the mixture was centrifuged to settle the cores. Then, the cores were purified by dispersing them in hexane and coagulating with acetone. The purification was repeated two times. The absorption spectrum of the resultant CdSe cores had a peak at 401 nm, which, according to Ref. 18, corresponds to a core diameter of 1.5 nm. Their PL spectrum had a peak at 442 nm and a full width at half maximum (FWHM) of 30 nm.

The next problem consisted in that the rapid termination of synthesis leaved considerable amounts of unreacted precursors in the mixture. Cadmium precursors, in the forms of cadmium alkyl phosphonates and carboxylates, cannot be totally removed by the dispersion/coagulation procedure, because they are adsorbed on the NC surface [19], the process being further facilitated by the small size and, hence, large relative surface area of the nanocrystals. Moreover, these remaining precursors are involved in reaction during the subsequent formation of the shell, either causing additional growth of the core or being included in the shell and disturbing its designed stoichiometry.

This problem was addressed by additional purification of the CdSe cores by gel permeation chromatography (GPC) [19] using the SX-1 cross-linked polystyrene beads (BIO-RAD) as the
stationary carrier phase. In this method, QD cores rapidly migrate along the stationary phase, while low-molecular-weight precursors are removed as a result of retention in the pores of the carrier [19].

In order to estimate how this additional purification improves the quality of the resultant QDs, we compared the optical characteristics of the core-shell QDs grown with or without GPC-purification of the cores. The results are shown in Table 1 and Figure 1.

<figure><img src="image_4.png" /><figcaption>**Figure 1.** Absorption spectra (a) and fluorescence spectra (b) of quantum dots with different shell structures and procedures for nanoparticles isolation and purification.</figcaption></figure>

The CdSe cores purified by the dispersion/coagulation method alone (Sample 1 in Table 1) or dispersion/coagulation followed by GPC (Sample 2) were coated with three monolayers of ZnS. We used the method of successive ion layer adsorption and reaction (SILAR) [20,21], because it allows layer-by-layer coating with a predetermined number of layers. Some GPC-purified cores were coated with a multicomponent (ZnS/CdS/ZnS) shell three monolayers in thickness (Sample 3). This type shell was earlier shown [17] to ensure an enhanced charge localization, thereby substantially increasing the PL QY. The final size of the CdSe/ZnS and CdSe/ZnS/CdS/ZnS QDs was less than 4 nm.

The incomplete removal of cadmium precursors from the solution of CdSe cores led to the formation of an inner CdS layer or a layer of a more complex and varying composition (CdₓZn₁-xS) in the shells of QDs in Sample 1. As can be seen from Table 1 and Figure 1, this has "blurred" the excitonic transition due to the formation of several types of QDs, which is expressed in a wide FWHM of both absorbance and PL peaks. Sample 1 is also characterized by a 56-nm red shift of the PL peak. CdSe/ZnS QDs in Sample 2 are considerably more homogeneous, as evidenced by their more than 1.5-fold narrower PL band. In addition, the red shift of the PL peak is also smaller (37 nm). Thus, the additional GPC purification of CdSe cores has substantially improved the optical parameters of the resultant QDs.
As expected, CdSe/ZnS/CdS/ZnS QDs in Sample 3, which also are based on GPC-purified cores, were as homogeneous as Sample 2, as judged by the FWHM of their PL spectrum (Table 1). The multicomponent shell has ensured an improved charge carrier localization in the core and their better protection from the environment, which has resulted in a higher PL QY (90%). The large red shift of the PL band of these QDs (79 nm) is explained by the complex energy band structure of their multicomponent shell [3,17].

<table><caption>**Table 1.** Optical characteristic of quantum dots with different shell structures and procedures for nanoparticles isolation and purification.</caption><thead><tr><th>No.</th><th>Sample</th><th>Absorbance peak, nm / PL peak, nm / FWHM, nm</th><th>PL QY, %</th></tr></thead><tbody><tr><td>1</td><td>CdSe/ZnS</td><td>- / 498 / 73</td><td>63 (relative to Coumarin 102)</td></tr><tr><td>2</td><td>CdSe/ZnS, GPC-purified</td><td>449 / 479 / 46</td><td>68 (relative to Coumarin 102)</td></tr><tr><td>3</td><td>CdSe/ZnS/CdS/ZnS, GPC-purified</td><td>517 / 537 / 46</td><td>90 (relative to fluorescein)</td></tr></tbody></table>

Thus, the experimental results confirmed the efficiency of our new procedure for the synthesis of ultrasmall CdSe cores with rapid termination of the reaction and additional GPC purification of the cores. We plan to use the CdSe/ZnS and CdSe/ZnS/CdS/ZnS QDs designed in this study as fluorescent labels in next-generation nanoprobes for *in vivo* and *in vitro* bioimaging [22].

## Acknowledgements

This study was supported by the Ministry of Education and Science of the Russian Federation, State Contract no. 4.624.2014/K. We thank Mr. Vladimir Ushakov for the help in preparation of the manuscript.

This work was supported by Competitiveness Program of National Research Nuclear University MEPhI.

## References

[1] Klimov V, Ivanov S, Nanda J, Achermann M, Bezel I, McGuire J and Piryatinski A 2007 Nat. 447 441-6

[2] Vokhmintcev KV, Samokhvalov PS and Nabiev I 2016 Nano Today 11 189-211

[3] Samokhvalov P, Artemyev M and Nabiev I 2013 Chemistry - Eur. J. 19 1534-46

[4] Chen Y, Vela J, Htoon H, Casson J L, Werder DJ, Bussian DA, Klimov VI and Hollingsworth JA 2008 JACS 130 5026-7

[5] Boldt K, Kirkwood N, Beane G A and Mulvaney P 2013 Chem. Mat. 25 4731-8

[6] Cao G 2004 Nanostructures and Nanomaterials: Synthesis, Properties, and Applications ed S Chong and L Narayanan (London: Imperial College Press) 2nd edn

[7] Anikeeva PO, Halpert JE, Bawendi MG and Bulović V 2009 Nano Lett. 9 2532-6

[8] Rakovich TY, Mahfoud OK, Mohamed BM, Prina-Mello A, Crosbie-Staunton K, Van Den Broeck T, De Kimpe L, Sukhanova A, Baty D, Rakovich A, Maier SA, Alves F, Nauwelaers F, Nabiev I, Chames P and Volkov Y 2014 ACS NANO 8 5682-95

[9] Bobrovsky A, Mochalov K, Oleinikov V, Sukhanova A, Prudnikau A, Artemyev M, Shibaev V and Nabiev I 2012 Adv. Mater. 24 6216-22

[10] Brazhnik K, Sokolova Z, Baryshnikova M, Bilan R, Efimov A, Nabiev I and Sukhanova, A 2015 Nanomedicine: NBM 11 1065-75

[11] Artemyev M, Ustinovich E and Nabiev I 2009 J. Am. Chem. Soc. 131 8061-5

[12] Hafian H, Sukhanova A, Turini M, Chames P, Baty D, Pluot M, Cohen JHM, Nabiev I and Millot J-M 2014 Nanomed.: NBM 10 1701-9
[13] Ishimoto T, Ozawa T and Mori H 2011 Bioconj. Chem. 22 1136–44

[14] Hollingsworth JA 2013 Chem.Mat.: publication of the ACS 25 1318–31

[15] Harrell S M, McBride J R and Rosenthal S J 2013 Chem. Mat. 25 1199–210

[16] Kudera S, Zanella M, Giannini C, Rizzo A, Li Y, Gigli G, Cingolani R, Ciccarella G, Spahl W, Parak WJ and Manna L 2007 Adv. Mat. 19 548–52

[17] Samokhvalov P, Linkov P, Michel J, Molinari M and Nabiev I 2014 Colloid. Nanopart. Biomed. Appl. IX. Proceed. SPIE 8955 89550S

[18] Jasieniak J, Smith L, Embden JV, Mulvaney P and Califano M 2009 J. Phys. Chem. C 113 19468–74

[19] Shen Y, Gee MY, Tan R, Pellechia PJ and Greytak AB 2013 Chem. Mat. 25 2838–48

[20] Blackman B, Battaglia DM, Mishima TD, Johnson MB and Peng X 2007 Chem. Mat. 19 3815–21

[21] Hao J, Zhou J and Zhang C 2013 Chem. Comm. 49 6346

[22] Linkov P, Laronze-Cochard M, Sapi J, Sidorov LN and Nabiev I 2015 Phys. Proc. 73 216–20